Temperature-induced order-disorder structural phase transitions of two-dimensional isostructural hexamethylenetetramine co-crystals.
Chia, Tze Shyang; Quah, Ching Kheng; Acta crystallographica Section B, Structural science, crystal engineering and materials 73 (2017) 879–890; doi:10.1107/S2052520617009520

data_2311772
_publ_section_title
;
 Temperature-induced order-disorder structural phase transitions of
 two-dimensional isostructural hexamethylenetetramine co-crystals.
;
_journal_issue                   'Pt 5'
_journal_name_full
'Acta crystallographica Section B, Structural science, crystal engineering and materials'
_journal_page_first              879
_journal_page_last               890
_journal_paper_doi               10.1107/S2052520617009520
_journal_volume                  73
_journal_year                    2017
_chemical_formula_moiety         '2(C8 H8 O2), C6 H12 N4'
_chemical_formula_sum            'C22 H28 N4 O4'
_chemical_formula_weight         412.48
_chemical_name_systematic
;
Hexamethylenetetramine bis(4-methylbenzoic acid)
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2yn'
_space_group_name_H-M_alt        'P 1 21/n 1'
_atom_sites_solution_hydrogens   mixed
_audit_creation_method           SHELXL-2014/7
_cell_angle_alpha                90
_cell_angle_beta                 99.6957(12)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.1425(4)
_cell_length_b                   28.0850(18)
_cell_length_c                   12.1822(8)
_cell_measurement_reflns_used    9593
_cell_measurement_temperature    100.0(1)
_cell_measurement_theta_max      28.28
_cell_measurement_theta_min      2.90
_cell_volume                     2071.6(2)
_computing_cell_refinement       'SAINT (Bruker, 2009)'
_computing_data_collection       'APEX2 (Bruker, 2009)'
_computing_data_reduction        'SAINT (Bruker, 2009)'
_computing_molecular_graphics
;
SHELXTL (Sheldrick, 2008), Mercury (Macrae <i>et al.</i>, 2008)
;
_computing_publication_material
;
PLATON (Spek, 2009)
;
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXS-2013 (Sheldrick, 2008)'
_diffrn_ambient_temperature      100.0(1)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.973
_diffrn_measurement_device_type  'Bruker APEX Duo CCD area detector'
_diffrn_measurement_method       '\f and \w scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0447
_diffrn_reflns_av_unetI/netI     0.0263
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.973
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -8
_diffrn_reflns_limit_k_max       36
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_number            6265
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.973
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         28.308
_diffrn_reflns_theta_min         1.450
_exptl_absorpt_coefficient_mu    0.092
_exptl_absorpt_correction_T_max  0.967050
_exptl_absorpt_correction_T_min  0.884699
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   '(<i>TWINABS</i>; Sheldrick, 2012)'
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    1.323
_exptl_crystal_description       block
_exptl_crystal_F_000             880
_exptl_crystal_size_max          0.378
_exptl_crystal_size_mid          0.183
_exptl_crystal_size_min          0.128
_refine_diff_density_max         0.357
_refine_diff_density_min         -0.218
_refine_diff_density_rms         0.056
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.039
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     282
_refine_ls_number_reflns         4998
_refine_ls_number_restraints     2
_refine_ls_restrained_S_all      1.041
_refine_ls_R_factor_all          0.0619
_refine_ls_R_factor_gt           0.0471
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0557P)^2^+0.7009P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1107
_refine_ls_wR_factor_ref         0.1205
_reflns_Friedel_coverage         0.000
_reflns_number_gt                4100
_reflns_number_total             4998
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            gw5053sup1.cif
_cod_data_source_block           1533073
_cod_original_sg_symbol_H-M      'P 21/n'
_cod_database_code               2311772
_shelx_shelxl_version_number     2014/7
_shelx_estimated_absorpt_t_min   0.966
_shelx_estimated_absorpt_t_max   0.988
_exptl_absorpt_special_details
; 
The crystal was placed in the cold stream of an Oxford Cryosystems 
Cobra open-flow nitrogen cryostat (Cosier & Glazer, 1986) operating 
at 100.0 (1) K.
;
_shelx_res_checksum              13594
_shelx_hkl_checksum              22648